Twodimensional ternary locally resonant phononic crystals with a comblike coating


 Philip Riley
 1 years ago
 Views:
Transcription
1 Twodimensional ternary locally resonant phononic crystals with a comblike coating YanFeng Wang, YueSheng Wang,*, and Litian Wang Institute of Engineering Mechanics, Beijing Jiaotong University, Beijing, 00044, China Department of Mechanical Engineering, Østfold University College, Halden, 757, Norway Abstract Twodimensional ternary locally resonant phononic crystals can be used for vibration control and noise insulation in the low (even audible) frequency range. They used to consist of cylindrical scatterers with uniform coatings in their exterior. An alternative coating scheme with a comblike profile is proposed and investigated in this paper. The band structures are calculated by using the finite element method. It is found that a complete bandgap at a significantly low frequency, the wavelength of which is more than 0 times of the lattice constant, can be induced. The mechanism for such a change is suggested by using an equivalent springmass model based on analyzing the eigen modes at the bandgap edges. Numerical results and the results predicted by the springmass model are coherent. * Corresponding author: (Y. S. Wang)
2 . Introduction A growing interest has been focused on the periodic, elastic structures, called phononic crystals (PCs) []. The PCs, composed of two or more different kind of materials with different mechanical properties and mass densities, may exhibit bandgaps, within which the propagation of elastic or acoustic waves is prohibited. Two mechanisms may give rise to bandgaps, one is the Bragg scattering, and the other is the local resonance []. The latter can induce a complete bandgap at a frequency which is lower by two order of the magnitude than the former one. So the locally resonant PCs may have potential applications in the control of noise or vibration at low frequencies [3]. So far, various kinds of locally resonant PCs have been investigated [5]; and some equivalent analytical models are developed to evaluate the resonant frequencies or the lowest bandgap [68]. Wang et al. [7] examined the bandgap edge modes of the ternary locally resonant PCs, which are composed of lead spheres (solid cores) coated by silicon rubber (soft coatings) and embedded in hard epoxy (matrix). At the lower edge of the bandgap, the core oscillates as a rigid sphere and the coating acts as springs. While at the upper edge of the bandgap, the core and the matrix oscillate in a reverse phase. Based on the analysis of the edge modes, they developed equivalent springmass models to predict the bandgap edges. In their model, only the tensile spring was considered. The tensile spring constant was calculated from the tensile elastic constant of the coating which was approximated as a plane layer [6] between the cylinder and the matrix. Their results showed that a bandgap at a much lower frequency might be obtained by decreasing the modulus of the coating with the decrease of the bandgap width. However, it is not easy to find a material with very small modulus. Another choice is to decrease the area or volume of the coating by introducing holes. In this paper, we propose a twodimensional PC with a comblike coating by breaking the uniform coating into N discrete pieces, see Fig. (a). The sectorial pieces with the central angle of ( N) are equispaced in azimuth and oriented in the radial direction. Each piece [Fig. (c)] can be regarded as a spring in vibration, where i is the angle formed by the center line of the ith piece and the vibration direction of the core and is given by
3 i ( i ) N. The objective is to introduce free surfaces on every sectorial piece and to reduce the effective modulus of the springs, which will lead to a lower resonant frequency.. Numerical Results The band structures and the edge modes at the bandgap edge modes of the proposed locally resonant PC with a comblike coating are calculated by using the finite element software COMSOL. The detailed process can be found in Ref. [9]. The proposed ternary locally resonant PC is composed of cylindrical metal cores coated by rubber and embedded in the polymer matrix in a square lattice. The material parameters are listed in Table I. The inner and outer radii of the coating are r and r, respectively. And the lattice constant is a. The band structures for the PC with a coating of 6 pieces are shown in Fig. (a). For comparison, the results for the PC with a uniform coating are also presented, see Fig. (b). Here the reduced frequency a ( c ) (with c t being the transverse wave velocity of the matrix) is used. It t is noted that a complete bandgap between the 3rd and 4th bands appears in the frequency range of for the comblike coating or for the uniform coating, respectively. By introducing the comblike coating, the bandgap is obviously lowered as expected. The wavelength of the wave inside the bandgap is more than 0 times of the lattice constant. The associated edge modes of the amplitude of the displacements are shown in Fig. 3. At the lower edge of the bandgap [Figs. 3(a) and 3(c)], the steel core oscillates holistically, while the matrix is still. The coating acting as springs linking the core and the matrix. At the upper edge of the bandgap [Figs. 3(b) and 3(d)], however, the matrix also oscillates, in a reverse phase to the vibration of the steel core. Thus, similar to that in Ref. [7], equivalent 'massspringfixture' and 'massspringmass' models can be developed to represent these vibration modes, which will be discussed in detail in the next section. For the comblike coating, each piece plays different roles in vibration: some as tensile springs, some as shear springs, and the rest as a combination of both. The shear deformation of the comblike coating reduces the effective stiffness, and thus results in a lower bandgap. The variation of the bandgap edges with the piece number (N) is shown in Fig. 4. The results for the PC with a uniform coating (N=0) are also marked in the figure. With the increase of N in Fig. 4(a) (r /a=0.7), the lower edge of the bandgap first decreases quickly and then tends to a fixed value ( ); and the upper edge of the bandgap first 3
4 decreases sharply, then increases, and finally decreases in the same manner as the lower edge of the bandgap. The bandgap nearly disappears when N=, then enlarges again at N=3 and finally nearly unchanged ( ) with N increasing. To understand the narrowing or disappearing of the bandgap at N=, we illustrate the eigen modes of the amplitude of the displacements for PC with the coating of two pieces in Fig. 5. It is noted that the lower edge mode is similar to that of the uniform coating. While at the upper edge of the bandgap, the steel core and the matrix oscillate in a reverse phase along the direction without the coating pieces. So in this case, different from that of the lower edge, the coating acts as shear springs with small effective stiffness, which reduces the eigen frequency of the upper edge of the bandgap significantly, and hence the width of the bandgap. For comparison, we calculate the band structure of the PC with a 'virtual' uniform coating, of which the elastic modulus is a half of rubber (because the total area of the comblike coating is a half of that of the uniform coating). The two dotted lines in Fig.4 mark the lower/upper bandgap edges of the bandgap, and they are all higher than those for the comblike coating when N 3. So the descent of the bandgap edges by introducing the comblike coating is not only because of the decrease of the area of the coating, but also a consequence of the shear deformation of the comblike coating. Similar trend of the changes of the bandgap edges with N is shown in the case with larger steel cores (r /a=0.33), see Fig. 4(b). The most striking modification occurs when N=, where a small complete bandgap exists. A thinner coating exhibits a larger effective stiffness and thus results in opening of this small bandgap. When N 3, the complete bandgap tends to appear in the fixed frequency range of Equivalent springmass models The observations in preceding section cannot be explained simply on the basis of the original locally resonant model [] and the effective mass model [7] because of (a) topological difference of the coating layer and (b) introduction of free surfaces. In order to understand the mechanism of the bandgap generation and estimate the bandgap edges, we will propose an equivalent massspring model by taking both tensile and shear deformation, and the effect of the free surfaces into account. We first consider the PC with a uniform coating. Following the basic idea of Ref. [7], 4
5 there exists a standing point that is immoveable in the corresponding upper edge mode. Therefore the mass of the partial coating, which is mainly compressed or stretched, was divided into two parts and added to the mass of the two oscillators. However, in this paper, the mass of the whole coating is divided into two parts; and thus the effective masses of the two oscillators are, respectively, represented by m mcore mcoating ( ), () and m mmatrix mcoating ( ), () where m m ( m m ) ( m m ). These equations are indeed the modification of Eq. (0) in Ref. [7]. matrix coating core coating The coating is considered as a sum of many slenders (with the central angle d ) along the direction, see Fig. (b), where is the angle between each slender bar and the direction of the wave propagation. Different from Ref. [7], each slender bar is regarded as a tiny spring with both tensile and shear deformation. The effective tensile stiffness of a slender bar is and the effective shear stiffness is rd d t K C r r cos rd d s 44 K C r r sin, (3), (4) where C E( ) (( )( )) and C 44 E (( )) are the elastic constants for the isotropic elastic coating with E and being the Young's modulus and Poisson's ratio. Then the total effective stiffness of the entire coating may be obtained by considering contributions of all these tiny springs. The result is r( C C44) (d t d s) 0 r r K K K, (5) where the shear constant C 44 represents the contribution of the shear deformation of the coating. Thus, the eigen frequencies can be obtained by Km, (6) 5
6 for the lower edge of the bandgap, and K m K m, (7) for the upper edge of the bandgap. The above proposed model is different from the one developed in Ref. [7]. The latter one excludes the shear deformation of the coating. The results predicted by these two models are listed in Table II with the numbers in the brackets being the relative errors. Comparison of the numerical results from FEM and predicted results by these two models shows that both models can give satisfied predicted results for both lower and upper edges of the bandgap with small relative errors. The small mismatch between these two predicted results is mainly due to the fact that C C 44. That is to say, the two models give very similar results only in this particular case. The above proposed model is developed for the PC with a perfect coating. Then, can it be used for the PC with a comblike coating? To answer this question, we applied it directly to evaluate the lowest bandgap for the PC with a comblike coating. In this case, Eq. (5) should be rewritten as K N i i i (dk d K ). (8) Particular attention should be paid on the evaluation of the upper edge for N=, in which case the vibration mode is shown in Fig. 5(b) and thus ( i ). Evaluation of Eq. (8) with substantiation of Eqs. (3) and (4) yields t i s r( C C K ( r r) 44 ) (9) for N, and r CC44 ( C C44), upper edge of the bandgap r r K (0) r C C44 ( C C44), lower edge of the bandgap r r for N=. The difference between the lower and upper edges for N= is directly induced by the different roles of the coating in the vibration mode. It is noted that K, and therefore the 6
7 eigenfrequencies, are independent of N except N=. The predicted results from this model are shown as the thindashed and thinsolid lines in Fig. 4, which are unfortunately higher than the FEM results for the comblike coating. We note that area of the free surfaces increases with N increasing. Therefore, its influence on the total effective stiffness K might be the key fact to understand the variation of bandgap edges with N. It is known that the normal stress is zero on any free surface. Therefore, a thin 'surface layer' near the free surface is in the planestress state in each piece; while the central part is close to the planestrain state. However, in the above model, tensile stiffness ( ) of a slender bar is calculated through C [cf. Eq. (5)] by assuming the Kt planestrain state in the entire piece. This leads to the overestimation of the tensile spring constant of the comblike coating and thus yields the higher eigenfrequencies of the bandgap edges. In fact, for a uniform strain field along the rdirection, the stress in each piece is inhomogenous along the direction. Therefore, this should be a twodimensional problem. For simplicity, we will replace it by a onedimensional problem. In this sense, an improved onedimensional model will be developed to evaluate the total effective stiffness of the coating. The effective shear stiffness, immune to the free surface, is still given by Eq. (4). We will develop an improved model to calculate the effective tensile spring stiffness. For simplicity, we model each sectorial piece [Fig. (c)] as a strip infinitely long in zdirection ( z 0) with a l h rectangular crosssection, see Fig. 6. To determine the geometry map from a sectorial piece to a rectangular strip, we consider the following facts: The comblike coating tends to be a perfect coating when, in which case the whole coating, and therefore the rectangular strip, should be in the planestrain state [6]. That is to say, h when. On the other hand, when 0, each sectorial piece is very thin, in which case we should have h O( r ). Here we suggest the following relation between ( r, ) and (, l h) : l ( r r), h r. () [( ) ] which satisfies the above requirements. Then, the deformation of the sectorial piece along 7
8 rdirection can be simplified as onedimensional tension or compression of the rectangular strip along xaxis. In order to describe the inhomogeneous distribution of the stress, ( y), under a x uniform strain in xdirection, x, we assume that the Young's modulus is various as a function of y, which is denoted by E ( ) x y and sketched in Fig. 6. As mentioned before, the free surfaces (y=±h) are in the planestress state, i.e. y yx yz 0, which also implies that 0. The deformation along the zdirection is obviously uniform, therefore we xy zy have xz 0. Thus the stressstrain relation near the free surface is zx E, (at y=±h) () x x where E E h E. The central part far from the free surface is close to the ( ) ( ) x planestrain state. Therefore (0) E x should be between E' and C. If the strip is very thin ( hl 0 ), the whole strip is in the planestress state, and thus E ( y) E. If the strip is very thick (i.e. hl), the central part of the whole strip is nearly in the planestrain state with the stressstrain relation given by C. (3) x x x These facts imply that E ( ) x y should satisfy the following constraint conditions: Ex ( h) E, Ex ( y) E whenh l 0, Ex ( y0) C whenh l, (4) where y 0 is an arbitrary finite value. Based on the above analysis, we interpolate E ( ) x y by hl E ( y) E( C E)( y h)( e ). (5) x Applying Eq. (5) to the sectorial piece in Fig. (c), we have ( i ) r [( ) ] l Er ( ) E( C E )( )( e ) ( ) (6) in the cylindrical coordinate. 8
9 To verify the rationality of the proposed model, we calculate the strain energy of two configurations. One is a sectorial piece [Fig. (c)] subjected to an elongation along the rdirection. The strain energy is calculated by FEM. The other is the corresponding rectangular strip under the same elongation along xaxis. The strain energy is calculated with Eq. (5). The results for sectorial pieces with different central angles and those for their corresponding rectangular strips are illustrated in Fig. 7. An agreement is found between these two configurations, especially when the coating has more pieces. Finally, the associated effective tensile stiffness of each tiny spring is computed by rd d Kt Er( ) cos r r. (7) Then the total effective stiffness in Eq. (8) is modified as r K K K E C N i (d d ) ( 44) t s i i ( r r) N [( ) ] i r l ( i ) ( C E) e cos d. i i ( ) Unlike Eq. (9), the modified total effective stiffness varies with the piece number N. (8) By substituting Eq. (8) into Eqs. (6) and (7), we can evaluate the eigen frequencies at the bandgap edges, see Fig. 4, where the thickdashed and thicksolid lines represent the lower and upper edges of the bandgap, respectively. The agreement between the predicted results and the numerical ones is satisfactory. When N is big enough, the second part in Eq. (6) approaches to zero and we have Er ( ) E. (9) Then the total effective stiffness is simplified by eliminating the second part in Eq. (8), and we get ' r( E C K ) 44, (0) ( r r) which is independent of N. Thus the eigenfrequencies of the bandgap edges approach constants or 'fixed values' when N as mentioned before. Moreover, the numerical results for the PCs in a triangular lattice are also plotted in Fig.4. The steel core, the coating and their filling ratio are exactly the same as those in the 9
10 square lattice. The results confirm that the locally resonant gap is invariant with respect to the lattice symmetries []. In other words, the proposed model can evaluate the lowest bandgap for twodimensional locally resonant PC with a comblike coating regardless of the lattice symmetry. Another way to develop an equivalent springmass model is to model the comblike coating as an 'effective homogeneous perfect coating' of which the effective bulk and shear moduli [0] are obtained based on the equivalence of the strain energy. As indicated before, the shear modulus is uniform in a sectorial piece, immune to the free surfaces. Therefore the effective shear modulus is simply given by C /. () 44 The derivation of the effective bulk modulus, k, is cumbersome. We present the details in Appendix. The final result is with l and h given by Eq. (). Nh( r r ) r r k [ E ( C E )( e ) ], () 4 ' ' hl / r r The effective bulk modulus, normalized by the shear modulus of the coating, is shown in Fig. 8. As we can see, it decreases monotonously as the number of pieces increasing, as a main consequence of the decrease of the Young's modulus in Eq. (5). Meanwhile, replacing C with (k ) and C 44 with in Eq. (5), Eqs. (6) and (7) can be used to evaluate the bandgap edges, see Table III. The numbers in the brackets show the relative errors compared to the FEM results. Predicted results with these effective moduli by the model in Ref. [7], as well as those predicted by the modulus function in Eq. (6) are also presented for comparison. For a small piece number (N=4), the pieces distribute so sparsely that the comblike coating cannot be approximated as a 'perfect coating'. Then a big relative error is shown. For a big piece number (N=3), the pieces are evenly distribute, and we have a small relative error. Unfortunately, the bandgap edges evaluated by either the model of Eq. (5) or the one in Ref. [7] are still much underestimated. However the model of Eq. (5) or (6) can yield more accurate results. 0
11 4. Conclusions In summary, when a comblike coating is introduced to the ternary locally resonant PC, a complete bandgap at a lower frequency can be obtained, except for the case of a comblike coating with two pieces. This is due to the fact that the thin layers of the 'planestress' state near the free surface can decrease the effective stiffness of the coating. The width of this low bandgap, which is a little smaller than that for a uniform coating, is nearly unchanged with its center frequency getting slightly low when the piece number increases. An equivalent springmass model is proposed for a better understanding of the mechanism of the bandgap generation as well as accurate evaluation of the corresponding bandgap edges. The research is relevant to the design of locally resonant PCs which have the potential applications in wave or noise control in the low (even audible) frequency range. It is worthy to point out that this paper just provides a basic idea for the design of the locally resonant PCs with a comblike coating. Actually, a steel core coated with the comblike coating can be manufactured by wrapping the core with a thin layer of coating with many discrete pieces. The discrete piece can also be in other shape, such as parallelogram, trapezoid, etc. Distinguished features maybe expected with various comblike coatings. Acknowledgements The authors are grateful for the support from the National Natural Science Foundation of China (Grant No. 704), the National Basic Research Program of China (00CB7304) and the Oslofjord Research Fond of Norway (RFFOFJORES46898). The first author also acknowledges Rino Nilsen for fruitful discussion during his short visit at Fredrikstad. Appendix In this appendix, we show the process to calculate the effective bulk modus of the comblike coating based on the energy method. We consider the equivalence of the train energy between two states: one is a comblike coating with N pieces subjected to an elongation along the rdirection; the other is the corresponding 'effective homogeneous
12 perfect coating' with the effective bulk modulus k and the effective shear modulus under the same elongation along the rdirection. The effective shear modulus is given in Eq. (). Next we determine the effective bulk modulus k. Suppose that the comblike coating is sustained an elongation along the rdirection. Its strain energy can be calculated by the sum of the strain energy of N identical l h rectangular strips [Fig. 6] under the elongation of along the xaxis. The strain energy density in each strip is w x x d ( ) d 0 x x E 0 x y x x x ( ) l E y. (A) Then the strain energy of the comblike coating is l h Nh ' ' hl / W N w 0 dd x y [ E ( CE )( e )]. (A) h l Deformation of an 'effective homogeneous perfect coating' under the elongation along the rdirection is an axisymmetric elastic problem of which the displacement field can be generally written as ur Dr D r [] where D and D are determined by the boundary condition. Suppose that the inner boundary of the coating is fixed, and the outer boundary is subjected to a displacement. We can have D r ( r r ) and D Dr. Then the strain energy density in the 'effective homogeneous perfect coating' is w And the total strain energy is r )] r rd r d [4 ( 0 k r r ( r r ). (A3) r W w rdd r [4k ( r r )]. (A4) r 0 r r r Equating the strain energy and W, we get the effective bulk modulus as W Nh( r r ) r r k [ E ( C E )( e ) ]. (A5) 4 ' ' hl / r r
13 Reference list [] Kushwaha M S, Halevi P, Dobrzynski L, and DjafariRouhani B 993 Phys. Rev. Lett. 7 0 [] Liu Z Y, Chan C T, and Sheng P 00 Phys. Rev. B [3] Ho K M, Cheng C K, Yang Z, Zhang X X, and Sheng P 003 Appl. Phys. Lett [4] Liu Z Y, Zhang X X, Mao Y W, Zhu Y Y, Yang Z Y, Chan C T, and Sheng P 000 Science [5] Hsu J C and Wu T T 007 Appl. Phys. Lett [6] Hirsekorn M 004 Appl. Phys. Lett [7] Wang G, Shao L H, Liu Y Z, and Wen J H 006 Chin. Phys [8] Wang Y F and Wang Y S 03 J Vib. Acoust [9] Wang Y F, Wang Y S, and Su X X 0 J. Appl. Phys [0] Wu Y, Lai Y, and Zhang Z Q 007 Phys. Rev. B [] Timoshenko S and Goodier J N (nd ed) 95 Theory of Elasticity (New York: McGrawHill) 3
14 Table captions Table I. Elastic parameters of the materials. Table II. Normalized Bandgap edges ( a ( c ) ) predicted by equivalent models for PC t with a uniform coating under different geometrical parameters. Table III. Normalized Bandgap edges ( a ( c ) ) for PC with a comblike coating t evaluated by using the effective bulk and shear moludi (r /a=0.7 and r /a=0.4). Figure captions Fig. Configurations of the ternary PC with a comblike coating (a) and a uniform coating (b). The white part in panel (b) is vacuum. Panel (c) shows a sectorial piece of the comblike coating in panel (a). Fig. Band structures of the PC with (a) a comblike coating of 6 pieces and (b) a uniform coating in a square lattice, where r /a=0.7 and r /a=0.4. Fig. 3 Vibration modes of the amplitude of the displacements at the bandgap edges marked in Fig.. Panels (a)(d) correspond to points SS4, respectively. Fig.4 Variations of bandgap edges with the number of the comblike coating for r /a=0.4 and r /a=0.7 (a) or r /a=0.33 (b). The scattered symbols represent the numerical results; and the solid and dashed lines represent the analytical results. The two dotted lines represent the results for PC with a uniform coating, the modulus of which is a half of rubber. ( ) Lower edge for a square (triangular) lattice; ( ) Upper edge for a square (triangular) lattice. ( ) Lower edge evaluated by using Er ( )(C ); ( ) Upper edge evaluated by using Er ( )(C ). Fig.5 Vibration modes of the amplitude of the displacements at the lower edge (a) and the upper edge (b) for PC with a coating of two pieces. 4
15 Fig.6 Explanation of the calculation method of parameters in the proposed model for a l h rectangular strip with l ( r r) and h r, which corresponds to the [( ) ] sectorial piece in Fig. (c) Fig.7 Strain energy versus the central angle for one sectorial piece and its corresponding rectangular strip under the same elongation. Fig.8 Variations of the normalized effective bulk modulus with the piece number of the comblike coating for r /a=0.4. 5
16 Table I. Elastic parameters of the materials. Materials Core Coating Matrix Mass density, [kg/m 3 ] Young's modulus, E [Pa] Poisson's ratio,
17 Table II. Normalized Bandgap edges ( a ( c ) ) predicted by equivalent models for PC t with a uniform coating under different geometrical parameters. Geometry r /a=0.7 and r /a=0.4 r /a=0.33 and r /a=0.4 Bandgap edges Lower edge Upper edge Lower edge Upper edge FEM results Present model [Eq. (5)] (.3%) 0.34 (3.%) (.6%) 0.09 (.4%) Model in Ref. [7] (.5%) 0.35 (3.8%) (.4%) 0.09 (.4%) 7
18 Table III. Normalized Bandgap edges ( a ( c ) ) for PC with a comblike coating t evaluated by using the effective bulk and shear moludi (r /a=0.7 and r /a=0.4). Piece number N=4 N=3 Bandgap edges Lower edge Upper edge Lower edge Upper edge FEM results Present model [Eq. (6)] (0%) 0.06(%) 0.064(%) 0.050(4%) Present model [Eq. (5)]* 0.07(34%) (35%) 0.003(4%) 0.040(6%) Model in Ref. [7] 0.004(40%) (4%) 0.075(34%) (36%) *Note: C and C 44 in Eq. (5) are replaced by ( k ) and, respectively. 8
19 d 0 (Vibration direction) r r r r (a) (b) ( r r) i i r d (c) (Center line) i 0 (Vibration direction) Fig. Configurations of the ternary PC with a comblike coating (a) and a uniform coating (b). The white part in panel (b) is vacuum. Panel (c) shows a sectorial piece of the comblike coating in panel (a). 9
20 0.0 (a) 0.5 ac t S S 0.00 M X M Redeced wave vector 0.0 (b) 0.5 ac t 0.0 S4 S M X M Reduced wave vector Fig. Band structures of the PC with (a) a comblike coating of 6 pieces and (b) a uniform coating in a square lattice, where r /a=0.7 and r /a=0.4. 0
21 (a) (b) (c) (d) Fig. 3 Vibration modes of the amplitude of the displacements at the bandgap edges marked in Fig.. Panels (a)(d) correspond to points SS4, respectively.
22 0.5 (a) 0.0 ac t N 0.0 (b) 0.5 ac t N Fig.4 Variations of bandgap edges with the piece number of the comblike coating for r /a=0.4 and (a) r /a=0.7 or (b) r /a=0.33. The scattered symbols represent the numerical results; and the solid and dashed lines represent the analytical results. The two dotted lines represent the results for PC with a uniform coating, the modulus of which is a half of rubber. ( ) Lower edge for a square (triangular) lattice; ( ) Upper edge for a square (triangular) lattice. ( ) Lower edge evaluated by using Er ( )(C ); ( ) Upper edge evaluated by using Er ( )(C ).
23 (a) (b) Fig.5 Vibration modes of the amplitude of the displacements at the lower edge (a) and the upper edge (b) for PC with a coating of two pieces. 3
24 Free surface y h z y ' E C Ex ( y) x yz zy z zx yx xy xz x l Fig.6 Explanation of the calculation method of parameters in the proposed model for a l h rectangular strip with l ( r r) and h r, which corresponds to the [( ) ] sectorial piece in Fig.(c). 4
25 Strain energy (J) r /a=0.4 Numerical result for r /a=0.33 Predicted result for r /a=0.33 Numerical result for r /a=0.7 Predicted result for r /a= Fig.7 Strain energy versus the central angle for one sectorial piece and its corresponding rectangular strip under the same elongation. 5
26 4 3 r /a=0.7 r /a=0.33 k/c N Fig.8 Variations of the normalized effective bulk modulus with the piece number of the comblike coating for r /a=0.4. 6
EMA 3702 Mechanics & Materials Science (Mechanics of Materials) Chapter 2 Stress & Strain  Axial Loading
MA 3702 Mechanics & Materials Science (Mechanics of Materials) Chapter 2 Stress & Strain  Axial Loading MA 3702 Mechanics & Materials Science Zhe Cheng (2018) 2 Stress & Strain  Axial Loading Statics
More informationNoise Shielding Using Acoustic Metamaterials
Commun. Theor. Phys. (Beijing, China) 53 (2010) pp. 560 564 c Chinese Physical Society and IOP Publishing Ltd Vol. 53, No. 3, March 15, 2010 Noise Shielding Using Acoustic Metamaterials LIU Bin ( Ê) and
More informationComplete band gaps in twodimensional phononic crystal slabs
Complete band gaps in twodimensional phononic crystal slabs A. Khelif, 1 B. Aoubiza, 2 S. Mohammadi, 3 A. Adibi, 3 and V. Laude 1 1 Institut FEMTOST, CNRS UMR 6174, Université de FrancheComté, Besançon,
More informationQuestion 9.1: A steel wire of length 4.7 m and crosssectional area 3.0 10 5 m 2 stretches by the same amount as a copper wire of length 3.5 m and crosssectional area of 4.0 10 5 m 2 under a given load.
More informationClass XI Chapter 9 Mechanical Properties of Solids Physics
Book Name: NCERT Solutions Question : A steel wire of length 4.7 m and crosssectional area 5 3.0 0 m stretches by the same 5 amount as a copper wire of length 3.5 m and crosssectional area of 4.0 0 m
More informationClass XI Physics. Ch. 9: Mechanical Properties of solids. NCERT Solutions
Downloaded from Class XI Physics Ch. 9: Mechanical Properties of solids NCERT Solutions Page 242 Question 9.1: A steel wire of length 4.7 m and crosssectional area 3.0 10 5 m 2 stretches by the same amount
More informationMethod for retrieving effective properties of locally resonant acoustic metamaterials
Method for retrieving effective properties of locally resonant acoustic metamaterials Vladimir Fokin, Muralidhar Ambati, Cheng Sun, and Xiang Zhang* Nanoscale Science and Engineering Center, University
More informationQuestion 9.1: Answer. Length of the steel wire, L 1 = 4.7 m. Area of crosssection of the steel wire, A 1 = m 2
Question 9.1: A steel wire of length 4.7 m and crosssectional area 3.0 10 5 m 2 stretches by the same amount as a copper wire of length 3.5 m and crosssectional area of 4.0 10 5 m 2 under a given load.
More informationControlling elastic wave with isotropic transformation materials
Controlling elastic wave with isotropic transformation materials Zheng Chang, Jin Hu, a, Gengkai Hu, b, Ran Tao and Yue Wang School of Aerospace Engineering, Beijing Institute of Technology, 0008,Beijing,
More informationBand Gaps in a Multiresonator Acoustic Metamaterial
G. L. Huang Department of Systems Engineering, University of Arkansas at Little Rock, Little Rock, AR 7 email: glhuang@ualr.edu C. T. Sun School of Aeronautics and Astronautics, Purdue University, W.
More informationMetadamping: An emergent phenomenon in dissipative metamaterials
Metadamping: An emergent phenomenon in dissipative metamaterials Mahmoud I. Hussein and Michael J. Frazier Department of Aerospace Engineering Sciences, University of Colorado Boulder, Boulder, CO 80309
More informationGraduate School of Engineering, Kyoto University, Kyoto daigakukatsura, Nishikyoku, Kyoto, Japan.
On relationship between contact surface rigidity and harmonic generation behavior in composite materials with mechanical nonlinearity at fibermatrix interface (Singapore November 2017) N. Matsuda, K.
More informationEFFECT OF ELLIPTIC OR CIRCULAR HOLES ON THE STRESS DISTRIBUTION IN PLATES
EFFECT OF ELLIPTIC OR CIRCULAR HOLES ON THE STRESS DISTRIBUTION IN PLATES OF WOOD OR PLYWOOD CONSIDERED AS ORTHOTROPIC MATERIALS Information Revied and Reaffirmed March 1956 No. 1510 EFFECT OF ELLIPTIC
More informationQuestion Figure shows the strainstress curve for a given material. What are (a) Young s modulus and (b) approximate yield strength for this material?
Question. A steel wire of length 4.7 m and crosssectional area 3.0 x 105 m 2 stretches by the same amount as a copper wire of length 3.5 m and crosssectional area of 4.0 x 105 m 2 under a given load.
More informationDual phononic and photonic band gaps in a periodic array of pillars deposited on a membrane
Excerpt from the Proceedings of the COMSOL Conference 010 Paris Dual phononic and photonic band gaps in a periodic array of pillars deposited on a membrane Y. Pennec, Y. El Hassouani, C. Li, B. Djafari
More informationModule 7: Micromechanics Lecture 29: Background of Concentric Cylinder Assemblage Model. Introduction. The Lecture Contains
Introduction In this lecture we are going to introduce a new micromechanics model to determine the fibrous composite effective properties in terms of properties of its individual phases. In this model
More informationSUPPLEMENTARY FIGURES
SUPPLEMENTARY FIGURES Supplementary Figure 1 Tuning the eigenfrequencies of the translational modes. A cutaway drawing of the metamaterial unit cell is shown in a. Here, h s denotes the silicone rubber
More informationChapter 3. Load and Stress Analysis
Chapter 3 Load and Stress Analysis 2 Shear Force and Bending Moments in Beams Internal shear force V & bending moment M must ensure equilibrium Fig. 3 2 Sign Conventions for Bending and Shear Fig. 3 3
More informationBuckling Behavior of 3D Randomly Oriented CNT Reinforced Nanocomposite Plate
Buckling Behavior of 3D Randomly Oriented CNT Reinforced Nanocomposite Plate Outline Introduction Representative Volume Element (RVE) Periodic Boundary Conditions on RVE Homogenization Method Analytical
More informationInterfacial effects in electromagnetic coupling within piezoelectric phononic crystals
Acta Mech Sin (29) 25:95 99 DOI 1.17/s149821y RESEARCH PAPER Interfacial effects in electromagnetic coupling within pieoelectric phononic crystals F. J. Sabina A. B. Movchan Received: 14 July 28 / Accepted:
More informationFREE VIBRATION ANALYSIS OF THIN CYLINDRICAL SHELLS SUBJECTED TO INTERNAL PRESSURE AND FINITE ELEMENT ANALYSIS
FREE VIBRATION ANALYSIS OF THIN CYLINDRICAL SHELLS SUBJECTED TO INTERNAL PRESSURE AND FINITE ELEMENT ANALYSIS J. Kandasamy 1, M. Madhavi 2, N. Haritha 3 1 Corresponding author Department of Mechanical
More informationA novel type of transverse surface wave propagating in a layered structure consisting of a piezoelectric layer attached to an elastic halfspace
Acta Mech Sin 2010 26:417 423 DOI 10.1007/s1040901003365 RESEARCH PAPER A novel type of transverse surface wave propagating in a layered structure consisting of a piezoelectric layer attached to an
More informationModelling and Simulation of Acoustic Wave Propagation in. Locally Resonant Sonic Materials
Special session: Ultrasonic Modelling INVITED PAPER Version 1, 06/04/2003 Modelling and Simulation of Acoustic Wave Propagation in Locally Resonant Sonic Materials M. Hirsekorn a, P. P. Delsanto a, N.
More informationChapter 5 CENTRIC TENSION OR COMPRESSION ( AXIAL LOADING )
Chapter 5 CENTRIC TENSION OR COMPRESSION ( AXIAL LOADING ) 5.1 DEFINITION A construction member is subjected to centric (axial) tension or compression if in any cross section the single distinct stress
More informationEE C247B ME C218 Introduction to MEMS Design Spring 2017
247B/M 28: Introduction to MMS Design Lecture 0m2: Mechanics of Materials CTN 2/6/7 Outline C247B M C28 Introduction to MMS Design Spring 207 Prof. Clark T. Reading: Senturia, Chpt. 8 Lecture Topics:
More informationAcoustic metamaterials in nanoscale
Acoustic metamaterials in nanoscale Dr. Ari Salmi www.helsinki.fi/yliopisto 12.2.2014 1 Revisit to resonances Matemaattisluonnontieteellinen tiedekunta / Henkilön nimi / Esityksen nimi www.helsinki.fi/yliopisto
More informationSolid State Theory Physics 545
olid tate Theory hysics 545 Mechanical properties of materials. Basics. tress and strain. Basic definitions. Normal and hear stresses. Elastic constants. tress tensor. Young modulus. rystal symmetry and
More information1. A pure shear deformation is shown. The volume is unchanged. What is the strain tensor.
Elasticity Homework Problems 2014 Section 1. The Strain Tensor. 1. A pure shear deformation is shown. The volume is unchanged. What is the strain tensor. 2. Given a steel bar compressed with a deformation
More informationA simple planestrain solution for functionally graded multilayered isotropic cylinders
Structural Engineering and Mechanics, Vol. 24, o. 6 (2006) 000000 1 A simple planestrain solution for functionally graded multilayered isotropic cylinders E. Pan Department of Civil Engineering, The
More informationMECHANICS OF MATERIALS
Third E CHAPTER 2 Stress MECHANICS OF MATERIALS Ferdinand P. Beer E. Russell Johnston, Jr. John T. DeWolf Lecture Notes: J. Walt Oler Texas Tech University and Strain Axial Loading Contents Stress & Strain:
More informationMaterials: engineering, science, processing and design, 2nd edition Copyright (c)2010 Michael Ashby, Hugh Shercliff, David Cebon.
Modes of Loading (1) tension (a) (2) compression (b) (3) bending (c) (4) torsion (d) and combinations of them (e) Figure 4.2 1 Standard Solution to Elastic Problems Three common modes of loading: (a) tie
More informationIntroduction to Continuous Systems. Continuous Systems. Strings, Torsional Rods and Beams.
Outline of Continuous Systems. Introduction to Continuous Systems. Continuous Systems. Strings, Torsional Rods and Beams. Vibrations of Flexible Strings. Torsional Vibration of Rods. BernoulliEuler Beams.
More informationMacroscopic Elastic Constitutive Relationship of CastinPlace HollowCore Slabs
Macroscopic Elastic Constitutive Relationship of CastinPlace HollowCore Slabs JingZhong Xie 1 Abstract: The macroscopic Poisson ratio and elastic moduli of the castinplace hollowcore slab are researched
More informationThe Relationship between the Applied Torque and Stresses in PostTension Structures
ECNDT 6  Poster 218 The Relationship between the Applied Torque and Stresses in PostTension Structures Fui Kiew LIEW, Sinin HAMDAN * and Mohd. Shahril OSMAN, Faculty of Engineering, Universiti Malaysia
More information6.4 A cylindrical specimen of a titanium alloy having an elastic modulus of 107 GPa ( psi) and
6.4 A cylindrical specimen of a titanium alloy having an elastic modulus of 107 GPa (15.5 10 6 psi) and an original diameter of 3.8 mm (0.15 in.) will experience only elastic deformation when a tensile
More informationSchur decomposition in the scaled boundary finite element method in elastostatics
IOP Conference Series: Materials Science and Engineering Schur decomposition in the scaled boundary finite element method in elastostatics o cite this article: M Li et al 010 IOP Conf. Ser.: Mater. Sci.
More informationUNIT 1 STRESS STRAIN AND DEFORMATION OF SOLIDS, STATES OF STRESS 1. Define stress. When an external force acts on a body, it undergoes deformation.
UNIT 1 STRESS STRAIN AND DEFORMATION OF SOLIDS, STATES OF STRESS 1. Define stress. When an external force acts on a body, it undergoes deformation. At the same time the body resists deformation. The magnitude
More informationExample3. Title. Description. Cylindrical Hole in an Infinite MohrCoulomb Medium
Example3 Title Cylindrical Hole in an Infinite MohrCoulomb Medium Description The problem concerns the determination of stresses and displacements for the case of a cylindrical hole in an infinite elastoplastic
More informationTuesday, February 11, Chapter 3. Load and Stress Analysis. Dr. Mohammad Suliman Abuhaiba, PE
1 Chapter 3 Load and Stress Analysis 2 Chapter Outline Equilibrium & FreeBody Diagrams Shear Force and Bending Moments in Beams Singularity Functions Stress Cartesian Stress Components Mohr s Circle for
More informationMathematical Modeling of Displacements and Thermal Stresses in Anisotropic Materials (Sapphire) in Cooling
Mathematical Modeling of Displacements and Thermal Stresses in Anisotropic Materials (Sapphire) in Cooling Timo Tiihonen & Tero Tuovinen September 11, 2015 European Study Group with Industry, ESGI 112,
More informationUnit I  Properties of Matter
Unit I  Properties of Matter Elasticity: Elastic and plastic materials Hooke s law elastic behavior of a material stress  strain diagram factors affecting elasticity. Three moduli of elasticity Poisson
More informationSuperreflection and Cloaking Based on Zero Index Metamaterial
Superreflection and Cloaking Based on Zero Index Metamaterial Jiaming Hao, Wei Yan, and Min Qiu Photonics and Microwave ngineering, Royal Institute of Technology (KTH), lectrum 9, 164 4, Kista, Sweden
More informationCOMPRESSION AND BENDING STIFFNESS OF FIBERREINFORCED ELASTOMERIC BEARINGS. Abstract. Introduction
COMPRESSION AND BENDING STIFFNESS OF FIBERREINFORCED ELASTOMERIC BEARINGS HsiangChuan Tsai, National Taiwan University of Science and Technology, Taipei, Taiwan James M. Kelly, University of California,
More informationStability of Simply Supported Square Plate with Concentric Cutout
International OPEN ACCESS Journal Of Modern Engineering Research (IJMER) Stability of Simply Supported Square Plate with Concentric Cutout Jayashankarbabu B. S. 1, Dr. Karisiddappa 1 (Civil Engineering
More informationDynamic Mechanical Analysis (DMA) of Polymers by Oscillatory Indentation
Dynamic Mechanical Analysis (DMA) of Polymers by Oscillatory Indentation By Jennifer Hay, Nanomechanics, Inc. Abstract This application note teaches the theory and practice of measuring the complex modulus
More informationChapter 12. Static Equilibrium and Elasticity
Chapter 12 Static Equilibrium and Elasticity Static Equilibrium Equilibrium implies that the object moves with both constant velocity and constant angular velocity relative to an observer in an inertial
More informationA Piezoelectric Screw Dislocation Interacting with an Elliptical Piezoelectric Inhomogeneity Containing a Confocal Elliptical Rigid Core
Commun. Theor. Phys. 56 774 778 Vol. 56, No. 4, October 5, A Piezoelectric Screw Dislocation Interacting with an Elliptical Piezoelectric Inhomogeneity Containing a Confocal Elliptical Rigid Core JIANG
More information2.1 Strain energy functions for incompressible materials
Chapter 2 Strain energy functions The aims of constitutive theories are to develop mathematical models for representing the real behavior of matter, to determine the material response and in general, to
More informationFinite Element Analysis of Dynamic Properties of Thermally Optimal Twophase Composite Structure
Vibrations in Physical Systems Vol.26 (2014) Finite Element Analysis of Dynamic Properties of Thermally Optimal Twophase Composite Structure Abstract Maria NIENARTOWICZ Institute of Applied Mechanics,
More information6.730 Physics for Solid State Applications
6.730 Physics for Solid State Applications Lecture 5: Specific Heat of Lattice Waves Outline Review Lecture 4 3D Elastic Continuum 3D Lattice Waves Lattice Density of Modes Specific Heat of Lattice Specific
More informationPolarized pass band for longitudinal waves in solid. phononic crystal. Journal of Physics Communications. Related content PAPER OPEN ACCESS
Journal of Physics Communications PAPER OPEN ACCESS Polarized pass band for longitudinal waves in solid phononic crystals To cite this article: S K Han et al 2017 J. Phys. Commun. 1 055026 View the article
More informationBasic Energy Principles in Stiffness Analysis
Basic Energy Principles in Stiffness Analysis StressStrain Relations The application of any theory requires knowledge of the physical properties of the material(s) comprising the structure. We are limiting
More informationStressStrain Behavior
StressStrain Behavior 6.3 A specimen of aluminum having a rectangular cross section 10 mm 1.7 mm (0.4 in. 0.5 in.) is pulled in tension with 35,500 N (8000 lb f ) force, producing only elastic deformation.
More informationSTATICALLY INDETERMINATE STRUCTURES
STATICALLY INDETERMINATE STRUCTURES INTRODUCTION Generally the trusses are supported on (i) a hinged support and (ii) a roller support. The reaction components of a hinged support are two (in horizontal
More informationTHREE DIMENSIONAL STRESS ANALYSIS OF THE T BOLT JOINT
THREE DIMENSIONAL STRESS ANALYSIS OF THE T BOLT JOINT Víctor Martínez 1, Alfredo Güemes 2, Norbert Blanco 1, Josep Costa 1 1 Escola Politècnica Superior. Universitat de Girona. Girona, Spain (17071) 2
More informationBifurcation of Sound Waves in a Disturbed Fluid
American Journal of Modern Physics 7; 6(5: 995 http://www.sciencepublishinggroup.com/j/ajmp doi:.68/j.ajmp.765.3 ISSN: 368867 (Print; ISSN: 36889 (Online Bifurcation of Sound Waves in a Disturbed Fluid
More informationAnalysis of the geometrical dependence of auxetic behavior in reentrant structures by finite elements
Acta Mech. Sin. (2016) 32(2):295 300 DOI 10.1007/s1040901505342 RESEARCH PAPER Analysis of the geometrical dependence of auxetic behavior in reentrant structures by finite elements V. H. Carneiro 1
More informationPrecise method to control elastic waves by conformal mapping
THEORETICAL & APPLIED MECHANICS LETTERS 3, (3) Precise method to control elastic waves by conformal mapping Yongquan Liu, Wei Liu, and Xianyue Su a) LTCS and Department of Mechanics and Aerospace Engineering,
More informationGyroscopic matrixes of the straight beams and the discs
Titre : Matrice gyroscopique des poutres droites et des di[...] Date : 29/05/2013 Page : 1/12 Gyroscopic matrixes of the straight beams and the discs Summarized: This document presents the formulation
More informationRESEARCH PROJECT NO. 26
RESEARCH PROJECT NO. 26 DETERMINATION OF POISSON'S RATIO IN AD1 TESTING BY UNIVERSITY OF MICHIGAN REPORT PREPARED BY BELA V. KOVACS and JOHN R. KEOUGH \ MEMBER / / DUCTILE IRON \ SOCIETY Issued by the
More informationStrength of Material. Shear Strain. Dr. Attaullah Shah
Strength of Material Shear Strain Dr. Attaullah Shah Shear Strain TRIAXIAL DEFORMATION Poisson's Ratio Relationship Between E, G, and ν BIAXIAL DEFORMATION Bulk Modulus of Elasticity or Modulus of Volume
More informationPLAIN WEAVE REINFORCEMENT IN C/C COMPOSITES VISUALISED IN 3D FOR ELASTIC PARAMETRES
THE 19 TH INTERNATIONAL CONFERENCE ON COMPOSITE MATERIALS PLAIN WEAVE REINFORCEMENT IN C/C COMPOSITES VISUALISED IN 3D FOR ELASTIC PARAMETRES P. Tesinova Technical University of Liberec, Faculty of Textile
More informationApplication and analysis of phononic crystal energy harvesting devices
J. Eng. Technol. Educ. (013) 10(1): 186 March 013 Application and analysis of phononic crystal energy harvesting devices Department of Information Management, Chung Hwa University of Medical Technology.
More informationFinal Exam Solution Dynamics :45 12:15. Problem 1 Bateau
Final Exam Solution Dynamics 2 191157140 31012013 8:45 12:15 Problem 1 Bateau Bateau is a trapeze act by Cirque du Soleil in which artists perform aerial maneuvers on a boat shaped structure. The boat
More informationMECHANICAL PROPERTIES OF SOLIDS
Chapter Nine MECHANICAL PROPERTIES OF SOLIDS MCQ I 9.1 Modulus of rigidity of ideal liquids is (a) infinity. (b) zero. (c) unity. (d) some finite small nonzero constant value. 9. The maximum load a wire
More informationINFLUENCE OF FILL EFFECT ON PAYLOAD IN A LARGE LAUNCH VEHICLE FAIRING
INFLUENCE OF FILL EFFECT ON PAYLOAD IN A LARGE LAUNCH VEHICLE FAIRING Zheng Ling State Key Laboratory of Mechanical Transmission, College of Automotive Engineering, Chongqing University, Chongqing email:
More informationContinuum Mechanics. Continuum Mechanics and Constitutive Equations
Continuum Mechanics Continuum Mechanics and Constitutive Equations Continuum mechanics pertains to the description of mechanical behavior of materials under the assumption that the material is a uniform
More informationComputational models of diamond anvil cell compression
UDC 519.6 Computational models of diamond anvil cell compression A. I. Kondrat yev Independent Researcher, 5944 St. Alban Road, Pensacola, Florida 32503, USA Abstract. Diamond anvil cells (DAC) are extensively
More informationJeff Brown Hope College, Department of Engineering, 27 Graves Pl., Holland, Michigan, USA UNESCO EOLSS
MECHANICS OF MATERIALS Jeff Brown Hope College, Department of Engineering, 27 Graves Pl., Holland, Michigan, USA Keywords: Solid mechanics, stress, strain, yield strength Contents 1. Introduction 2. Stress
More informationAcoustic guiding and subwavelength imaging with sharp bending by sonic crystal
Acoustic guiding and subwavelength imaging with sharp bending by sonic crystal Bo Li, Ke Deng *, and Heping Zhao Department of Physics, Jishou University, Jishou 46, Hunan, hina A sharp bending scheme
More informationUNIT I SIMPLE STRESSES AND STRAINS
Subject with Code : SM1(15A01303) Year & Sem: IIB.Tech & ISem SIDDHARTH GROUP OF INSTITUTIONS :: PUTTUR Siddharth Nagar, Narayanavanam Road 517583 QUESTION BANK (DESCRIPTIVE) UNIT I SIMPLE STRESSES
More informationRAINBOWTRAPPING ABSORBERS FOR TRANSMISSION PROB LEMS: BROADBAND AND PERFECT SOUND ABSORBING PANELS.
RAINBOWTRAPPING ABSORBERS FOR TRANSMISSION PROB LEMS: BROADBAND AND PERFECT SOUND ABSORBING PANELS. Noé Jimenez, Vicent RomeroGarcía, Vincent Pagneux, and JeanPhilippe Groby Laboratoire d Acoustique
More informationMiao Boya and An Yu Department of Physics, Tsinghua University, Beijing , People s Republic of China
Localization in an acoustic cavitation cloud Miao Boya and An Yu Department of Physics, Tsinghua University, Beijing 100084, People s Republic of China Using a nonlinear sound wave equation for a bubbly
More informationModal analysis of an enclosure acoustic space based on spectrogeometric method
INTERNOISE 6 Modal analysis of an enclosure acoustic space based on spectrogeometric method Xianjie SHI ; Chunli LI ; Fengjun WANG 3 ; Wen L LI 4 Institute of Systems Engineering, China Academy of Engineering
More informationMODELLING AND MEASUREMENT OF BACKSCATTERING FROM PARTIALLY WATERFILLED CYLINDRICAL SHELLS
MODELLING AND MEASUREMENT OF BACKSCATTERING FROM PARTIALLY WATERFILLED CYLINDRICAL SHELLS Victor Humphrey a, Lian Sheng Wang a and Nisabha Jayasundere b a Institute of Sound & Vibration Research, University
More informationSound Propagation through Media. Nachiketa Tiwari Indian Institute of Technology Kanpur
Sound Propagation through Media Nachiketa Tiwari Indian Institute of Technology Kanpur LECTURE13 WAVE PROPAGATION IN SOLIDS Longitudinal Vibrations In Thin Plates Unlike 3D solids, thin plates have surfaces
More informationStructural Dynamics Lecture 4. Outline of Lecture 4. MultiDegreeofFreedom Systems. Formulation of Equations of Motions. Undamped Eigenvibrations.
Outline of MultiDegreeofFreedom Systems Formulation of Equations of Motions. Newton s 2 nd Law Applied to Free Masses. D Alembert s Principle. Basic Equations of Motion for Forced Vibrations of Linear
More informationDesign of a fastener based on negative Poisson's ratio foam adapted from
1 Design of a fastener based on negative Poisson's ratio foam adapted from Choi, J. B. and Lakes, R. S., "Design of a fastener based on negative Poisson's ratio foam", Cellular Polymers, 10, 205212 (1991).
More informationEsben Byskov. Elementary Continuum. Mechanics for Everyone. With Applications to Structural Mechanics. Springer
Esben Byskov Elementary Continuum Mechanics for Everyone With Applications to Structural Mechanics Springer Contents Preface v Contents ix Introduction What Is Continuum Mechanics? "I Need Continuum Mechanics
More informationEVALUATING RADIATION DAMPING OF SHALLOW FOUNDATIONS ON NONLINEAR SOIL MEDIUM FOR SOILSTRUCTURE INTERACTION ANALYSIS OF BRIDGES
EVALUATING RADIATION DAMPING OF SHALLOW FOUNDATIONS ON NONLINEAR SOIL MEDIUM FOR SOILSTRUCTURE INTERACTION ANALYSIS OF BRIDGES Abstract Jian Zhang 1 and Yuchuan Tang 2 The paper evaluates the radiation
More informationVIBRATION ANALYSIS OF TIEROD/TIEBOLT ROTORS USING FEM
VIBRATION ANALYSIS OF TIEROD/TIEBOLT ROTORS USING FEM J. E. Jam, F. Meisami Composite Materials and Technology Center Tehran, IRAN jejaam@gmail.com N. G. Nia Iran Polymer & Petrochemical Institute, Tehran,
More informationVIBRATION ENERGY FLOW IN WELDED CONNECTION OF PLATES. 1. Introduction
ARCHIVES OF ACOUSTICS 31, 4 (Supplement), 53 58 (2006) VIBRATION ENERGY FLOW IN WELDED CONNECTION OF PLATES J. CIEŚLIK, W. BOCHNIAK AGH University of Science and Technology Department of Robotics and Mechatronics
More informationChapter 6: Mechanical Properties of Metals. Dr. Feras Fraige
Chapter 6: Mechanical Properties of Metals Dr. Feras Fraige Stress and Strain Tension Compression Shear Torsion Elastic deformation Plastic Deformation Yield Strength Tensile Strength Ductility Toughness
More informationVORONOI APPLIED ELEMENT METHOD FOR STRUCTURAL ANALYSIS: THEORY AND APPLICATION FOR LINEAR AND NONLINEAR MATERIALS
The 4 th World Conference on Earthquake Engineering October 7, 008, Beijing, China VORONOI APPLIED ELEMENT METHOD FOR STRUCTURAL ANALYSIS: THEORY AND APPLICATION FOR LINEAR AND NONLINEAR MATERIALS K.
More informationNew Developments of Frequency Domain Acoustic Methods in LSDYNA
11 th International LSDYNA Users Conference Simulation (2) New Developments of Frequency Domain Acoustic Methods in LSDYNA Yun Huang 1, Mhamed Souli 2, Rongfeng Liu 3 1 Livermore Software Technology
More informationTesting and Analysis
Testing and Analysis Testing Elastomers for Hyperelastic Material Models in Finite Element Analysis 2.6 2.4 2.2 2.0 1.8 1.6 1.4 Biaxial Extension Simple Tension Figure 1, A Typical Final Data Set for Input
More informationOPTIMAL DESIGN OF COMPOSITE INSERTS FOR A HYBRID ULTRACENTRIFUGE ROTOR
18 TH INTERNATIONAL CONFERENCE ON COMPOSITE MATERIALS OPTIMAL DESIGN OF COMPOSITE INSERTS Hak Gu Lee 1*, Jisang Park 1, Ji Hoon Kim 1 1 Composite Materials Group, KIMS, Changwon, Korea * Corresponding
More informationL e c t u r e. D r. S a s s a n M o h a s s e b
The Scaled smteam@gmx.ch Boundary Finite www.erdbebenschutz.ch Element Method Lecture A L e c t u r e A1 D r. S a s s a n M o h a s s e b V i s i t i n g P r o f e s s o r M. I. T. C a m b r i d g e December
More informationSpherical cloaking with homogeneous isotropic multilayered structures
Spherical cloaking with homogeneous isotropic multilayered structures The MIT Faculty has made this article openly available. Please share how this access benefits you. Your story matters. Citation As
More informationNumerical study on scanning radiation acoustic field in formations generated from a borehole
Science in China Ser. G Physics, Mechanics & Astronomy 5 Vol.48 No. 47 56 47 Numerical study on scanning radiation acoustic field in formations generated from a borehole CHE Xiaohua 1, ZHANG Hailan 1,
More informationNumerical modelling of induced tensile stresses in rock in response to impact loading
Numerical modelling of induced tensile stresses in rock in response to impact loading M.T. Mnisi, D.P. Roberts and J.S. Kuijpers Council for Scientific and Industrial Research (CSIR): Natural Resources
More informationMechanical properties 1 Elastic behaviour of materials
MME131: Lecture 13 Mechanical properties 1 Elastic behaviour of materials A. K. M. B. Rashid Professor, Department of MME BUET, Dhaka Today s Topics Deformation of material under the action of a mechanical
More informationLocal Stresses in Belt Turnovers in Conveyor Belt
Local Stresses in Belt Turnovers in Conveyor Belt By: Conveyor Dynamics, Inc. personnel Conveyor Dynamics, Inc. 1111 W. Holly Street, Suite A Bellingham, WA 985 USA Abstract Belt turnovers are commonly
More informationAdvanced holographic nondestructive testing system for residual stress analysis
Advanced holographic nondestructive testing system for residual stress analysis Anatoli Kniazkov, Yuri Onischenko, George Dovgalenko, Gregory Salamo Laser Laboratory, Physics Department, University of
More informationAXISYMMETRIC ELASTICITY PROBLEM OF CUBIC QUASICRYSTAL *
Volume 9, Number April, 9963//9/9 CHINESE PHYSICS c Chin. Phys. Soc. AXISYMMETRIC ELASTICITY PROBLEM OF CUBIC QUASICRYSTAL * Zhou Wangmin and Fan Tianyou Research Center of Materials Science, Beijing
More informationChapter 13 ELASTIC PROPERTIES OF MATERIALS
Physics Including Human Applications 280 Chapter 13 ELASTIC PROPERTIES OF MATERIALS GOALS When you have mastered the contents of this chapter, you will be able to achieve the following goals: Definitions
More informationGame Physics. Game and Media Technology Master Program  Utrecht University. Dr. Nicolas Pronost
Game and Media Technology Master Program  Utrecht University Dr. Nicolas Pronost Soft body physics Soft bodies In reality, objects are not purely rigid for some it is a good approximation but if you hit
More informationMeasurement of Dynamic Viscoelasticity of FullSize Wood Composite Panels Using a Vibration Testing Method
Measurement of Dynamic Viscoelasticity of FullSize Wood Composite Panels Using a Vibration Testing Method Cheng Guan, a Houjiang Zhang, a, * John F. Hunt, b Lujing Zhou a and Dan Feng a The dynamic viscoelasticity
More informationChapter 5. Effects of Photonic Crystal Band Gap on Rotation and Deformation of Hollow Te Rods in Triangular Lattice
Chapter 5 Effects of Photonic Crystal Band Gap on Rotation and Deformation of Hollow Te Rods in Triangular Lattice In chapter 3 and 4, we have demonstrated that the deformed rods, rotational rods and perturbation
More informationPRELIMINARY PREDICTION OF SPECIMEN PROPERTIES CLT and 1 st order FEM analyses
OPTIMAT BLADES Page 1 of 24 PRELIMINARY PREDICTION OF SPECIMEN PROPERTIES CLT and 1 st order FEM analyses first issue Peter Joosse CHANGE RECORD Issue/revision date pages Summary of changes draft 241002
More information